Amine modification of calcium phosphate by low-pressure plasma for bone regeneration

Regeneration of large bone defects caused by trauma or tumor resection remains one of the biggest challenges in orthopedic surgery. Because of the limited availability of autograft material, the use of artificial bone is prevalent; however, the primary role of currently available artificial bone is restricted to acting as a bone graft extender owing to the lack of osteogenic ability. To explore whether surface modification might enhance artificial bone functionality, in this study we applied low-pressure plasma technology as next-generation surface treatment and processing strategy to chemically (amine) modify the surface of beta-tricalcium phosphate (β-TCP) artificial bone using a CH4/N2/He gas mixture. Plasma-treated β-TCP exhibited significantly enhanced hydrophilicity, facilitating the deep infiltration of cells into interconnected porous β-TCP. Additionally, cell adhesion and osteogenic differentiation on the plasma-treated artificial bone surfaces were also enhanced. Furthermore, in a rat calvarial defect model, the plasma treatment afforded high bone regeneration capacity. Together, these results suggest that amine modification of artificial bone by plasma technology can provide a high osteogenic ability and represents a promising strategy for resolving current clinical limitations regarding the use of artificial bone.

. Plasma polymerization system and characterization of plasma-polymerized films. (A) Schematic diagram of the pulsed-plasma deposition system used in this study. Samples were placed on the bottom metal electrode, which was powered by high-voltage bipolar pulse voltages with a peak-to-peak voltage of 2.2 kV. The power, repetition frequency, and duty cycle were 15 W, 5 kHz, and 1%, respectively. The plasma was generated from a gas mixture of CH 4 , N 2 , and He with flow rates of 10, 20, and 10 sccm, respectively, and a gas pressure of 70 Pa. (B) The atomic concentration ratios on a plasma-treated dense β-TCP disk surface (top) and those on an untreated dense β-TCP disk surface (bottom). More precise values are given in the main text. (C) The relative number of primary amines (-NH 2 ) among all atoms excluding hydrogen (left) and the number ratios of primary amines to C or N atoms (right) on the surface of the plasma-polymerized film deposited on a dense β-TCP disk. In (B,C), all measurements were triplicate. (D) The profiles of relative atomic concentrations along the center axis of a plasma-treated porous β-TCP disk, indicating plasma polymerization of the inner pore surfaces due to the penetration of plasma-generated deposition precursors through the interconnected pores from the plasma-treated disk surface. After a single side of a porous β-TCP disk was plasma-treated, it was cut in half through its center and the relative atomic concentrations were measured at 25 points along the center axis. The horizontal axis of the figure represents the position along the center axis measured from the plasma-exposed top surface of the disk. In each case above, the plasma treatment time was 30  www.nature.com/scientificreports/ sis; the marrow was flushed out using 10 ml of GM expelled from a syringe through a 21-gauge needle according to the previously described method 19 . The released cells were collected in two 100 mm culture dishes containing 15 ml of GM. The medium was changed after 24 h to remove hematopoietic cells and renewed twice weekly. Cultures were maintained in a humidified atmosphere of 95% air with 5% CO 2 at 37 °C. When the cells reached 80-90% confluency they were washed with phosphate-buffered saline (PBS) and trypsinized with 1% trypsinethylenediaminetetraacetic acid (EDTA). Following centrifugation for 5 min at 400g, the cells were resuspended and plated at a density of 3.6 × 10 4 /cm 2 . After again reaching confluency, cells were collected and stored at − 80 °C (Passage 1). Prior to in vitro experiments, stocked cells were thawed and resuspended in 15 ml of GM, then plated in a 100 mm dish and cultured for three days to reach 80-90% confluency (Passage 2).
Cell adhesion assay. A centrifugation cell adhesion assay was performed according to a published method 20 . Cell suspension (5 × 10 3 cells/35 μl GM) was gently dropped on each dense β-TCP disk surface to form a centroclinal water drop and incubated for 30 min in a 24 well culture plate to initiate adhesion. Then, 1 ml of PBS was gently added to each well containing a cell-adhered disk and macro fluorescence photos were taken with the Leica AF6000 Fluorescence Imaging System (Leica Microsystems, Wetzlar, Germany. Exposure: 1000 ms; Gain: 2.7; Binning 2 × 2; Magnification: 12.6×) to quantify the initial adherent cells. After this, the cell adhered disks were embedded into a 48-well culture plate containing 100 μl of Vaseline (KENEI Pharmaceutical Co., Ltd., Osaka, Japan) in each well. After filling each well with PBS, the plate was sealed with a sealing tape and set upside-down on a centrifuge (PlateSpinII, Kubota Corp., Tokyo, Japan) and centrifuged at 10g for 5 min to detach weakly adherent cells. After the centrifugation, the detached cells were slowly aspirated and each well was carefully filled with 200 μl of PBS. Macro fluorescence photos of the plate were taken again under the same conditions as those prior to the centrifugation. Automatic cell counting was performed with the macro fluorescence photos and ImageJ software 21 . The adhesion rate is defined as the ratio of the number of cells attached to the surface after centrifugation to that before centrifugation.

Morphology analysis of adhered cells.
Cell suspension (5 × 10 3 cells/35 μl GM) was gently dropped on dense β-TCP disks and incubated for 3 h in a 24-well culture plate to initiate adhesion. Then, the wells were slowly filled with 1 ml of GM, and the incubation was continued for another 24 h. Macro fluorescence photos of random areas of the culture wells containing incubated cells were then obtained. The open-source software CellProfiler (www. cellp rofil er. org) 22 was used for sorting cells and cell morphology analysis. In particular, the cell area was measured to quantify the spreading of attached BMSCs. Two cell-shape descriptors (circularity and solidity) were investigated; the circularity indicates the closeness of the cell shape to a perfect circle, and the solidity is an index to quantify the amount and size of concavities of the cell 23 : where A is the cell area and P is the perimeter.
where ConvexA is the area of the smallest convex hull that contains the cell.

Cell proliferation assay.
To balance the initial cell count of adherent cells on untreated and plasma-treated β-TCP disks, two different concentrations (5 × 10 3 cells/35 μl GM for the untreated group and 3 × 10 3 cells/35 μl GM for the plasma-treated group) of cell suspension were dropped on dense untreated and plasma-treated β-TCP disks in a 48-well plate. After incubating for 30 min, 500 μl of GM was slowly added to each well. At day 1, 3, 5, 7, 11, and 14, 50 μl of CCK-8 solution was added to each well and the plate was incubated for 2 h, then 100 μl of GM from each well was transferred into a 96-well plate. The optical density at 450 nm was measured using a spectrophotometer (Multiskan GO, Thermo Fisher Scientific).
Osteogenic differentiation assay. Cell suspension (2 × 10 4 cells/35 μl GM ) was dropped on dense β-TCP disks and incubated for 30 min in a 48-well plate to initiate adhesion. Then, 500 μl of GM was slowly added into each well, incubated for 24 h, and the culture medium was replaced with ODM for osteogenic differentiation. The subculture was maintained for another four days. After washing the disks twice with PBS, the attached cells were fixed using 500 μl of 4% paraformaldehyde (PFA) for ALP staining, according to the manufacturer's instructions (Promega Corp.). For ALP activity, 60 μl of M-PER was added to each well and the cells were detached from the disks using a mini scraper. After lysing the cells for 5 min, the supernatant was collected for ALP and total protein assays. An ALP activity unit was defined as the release of 1 nmol p-nitrophenol per min of incubation at 37 °C for each β-TCP disk. The total protein content of each sample was measured to standardize the ALP activity values. www.nature.com/scientificreports/ tissue. The plasma-treated and untreated β-TCP disks were implanted in the right and left defects, respectively. The rats were given free access to water and food after the surgery. The rats were sacrificed at postoperative 3 (n = 5) and 6 (n = 15) weeks by CO 2 inhalation. Microfocus computed tomography (micro-CT) and histological analyses were performed to evaluate new bone formation in the inner pores of porous β-TCP disks at 3 and 6 weeks postoperatively.

Microfocus computed tomography (micro-CT).
Harvested specimens were fixed in 10% buffered formalin, dehydrated and degreased using a graded ethanol series, and stored in 70% ethanol at 4 °C for micro-CT scanning (Skyscan 1272 micro-CT, Bruker, Kontich, Belgium), which was performed with the following parameters: camera binning = 2 × 2, source voltage = 80 kV, source current = 125 μA, image pixel size = 4 μm, rotation step = 0.6°, and filter = Al 1 mm. Image analysis was performed using CTAN software (Version 1.18.8.0+, Brucker). Micro-CT images of the specimens were compared with the results of histological evaluation of the specimens, discussed below, and the difference in image intensities between the newly formed bone and residual β-TCP was identified. Using this information, three-dimensional (3D) images of newly formed bones inside the porous β-TCP disks were reconstructed from the Micro-CT images of the specimens.
Histological evaluation. After micro-CT scanning, the specimens were demineralized using K-CX AT solution at 4 °C, cleared in xylene, and embedded in paraffin. Then, several sections of 4 μm thickness were cut off from the center of each specimen and stained with hematoxylin and eosin (H&E).
Statistical analysis. Statistical analysis was performed using GraphPad Prism version 7.04 for Windows (GraphPad Software, San Diego, CA, USA) applying the Mann-Whitney U test for non-parametric data, Student's or Welch's t-test for parametric data, and Wilcoxon matched-pairs signed-rank test for in vivo results. The values are presented as mean ± standard deviation (SD). The differences were considered statistically significant for p value < 0.05.

Ethic declarations. All animal work was approved by The Animal Experimental Committee of Osaka
University Graduate School of Medicine (01-070-000) and restrictedly followed ARRIVE guidelines and the National Institutes of Health Guide for the Care and Use of Laboratory Animals 24 .

Plasma polymerization on β-TCP disks. A bipolar pulsed-plasma deposition system developed at
Osaka University was used to perform plasma polymerization on dense and porous β-TCP disks. The schematic diagram of the system is given in Fig. 1A. The plasma was generated with a CH 4 /N 2 /He gas mixture with flow rates of 10, 20, and 10 sccm, respectively, and a gas pressure of 70 Pa. Methane (CH 4 ) was used to form an organic polymer, nitrogen (N 2 ) was to form amine groups, and helium (He) was to lower the plasma ignition voltage via Penning ionization. The plasma polymerization conditions used in this study, including the selection of the discharge gases and their mixing ratio, were selected to attain stable plasma discharge, a reasonable film deposition rate, and a relatively high amine concentration in the deposited film, using the gas species and discharge conditions that the authors are accustomed to operating the plasma system with for various other plasma polymerization applications 13,25 . Although the conditions used in this study were locally optimized (i.e., by varying the discharge parameters around those presented in this article), its global optimization with different combinations of organic and nitrogen-compound gaseous species has not been performed yet and is beyond the scope of the present study. The chemical compositions of the plasma-treated dense β-TCP disk obtained from XPS are Ca: P: O: C:N = 0.0 ± 0.0: 0.0 ± 0.0: 2.9 ± 0.2: 85.2 ± 0.1:11.9 ± 0.1 (at.%, n = 3). The N to C ratio of the deposited film is, therefore, N/C = 14.0%. The fact that neither Ca nor P was observed indicates that the deposited film was sufficiently thick (thicker than several nm at least). The observed small amount of O may indicate oxygen incorporated in the deposited film due to oxygen or water impurities off from the chamber walls of the plasma system during the plasma discharge or water (H 2 O) molecules attached to the polymer surfaces when the sample was exposed to ambient air. The results are summarized in Fig. 1B.
It is not easy to measure the thicknesses of deposited polymer films on β-TCP precisely as the roughness of β-TCP surfaces is far greater than the deposited film thickness. However, we surmise that the deposited polymer thickness on the β-TCP disk under the conditions described above (i.e., 30 min polymerization) was about 40 nm, based on the thickness of the plasma-polymerized film formed on a crystalline (100) Si surface under the same polymerization conditions, which was determined to be 44.2 ± 0.1 nm by ellipsometry.
The relative amount of primary amine (-NH 2 ) on a plasma-polymerized film surface was evaluated by the derivatization method 17,18 . Figure 1C shows the relative number of N atoms that form primary amine groups on the surfaces of plasma-polymerized films deposited on dense β-TCP disks 2 days after the film deposition. The left graph shows the atomic percentage of such N atoms among all surface atoms excluding hydrogen ( i.e., the The right graph shows the number ratios of primary amines to the surface C or N atoms, i.e., NH 2 /C = 1.6 ± 0.1 and NH 2 /N = 8.3 ± 0.5 (at.%, n = 3). It is seen here that about 8% of all deposited N atoms formed primary amines in the plasma-polymerized film. The remaining N atoms were most likely to form either secondary amines (-NH) or tertiary amines, i.e., nitrogen atoms bonded only with carbon atoms.
To observe whether the polymer depositing plasma penetrated the interconnected pores of artificial bone and coated their inner surfaces, we performed a cross-section analysis of a plasma-treated porous β-TCP disk. In this analysis, a single-side treated porous β-TCP disk was cut in half at the center and the cross sections were scanned with high-resolution XPS. The measurements were performed on 25 spots with a diameter of 100 μm along the center axis of the cross-section, as presented in Fig. 1D. The vertical and horizontal axes represent the percentages of atomic concentrations and the position along the center axis measured from the plasma-exposed top surface of the disk. We treated only a single side of the disk such that the penetration direction becomes clear. The untreated side of the disk was in direct contact with the electrode surface of the plasma system and not directly exposed to the plasma.
As seen in Fig. 1D, the C and N concentrations are the highest on the plasma-treated surface (i.e., at position 0) and decrease gradually toward the center. The fact that their concentrations slightly higher near the untreated side (i.e., near position 2 mm) suggests that some polymerizing gas entered from this side through a gap between the bottom surface of the disk and the electrode. Because the porosity of the disk is about 75% (i.e., 75% of the disk volume is void), we expect that the area ratio of the inner pore surface to the β-TCP bulk on the cross section is approximately 75 2/3 : 25 2/3 = 68: 32. We also note that the variation of atomic concentration ratios on the cross section is higher than the SD of the atomic concentration ratios on the untreated β-TCP surface given above. This is because of the random spatial distribution of inner pores, whose average diameter is 150 μm, inside the disk whereas the diameter of each measurement spot is 100 μm.
As discussed earlier, the atomic concentration ratios of untreated β-TCP were about Ca: P: O: C: N = 19: 11: 42: 28: 0 (at.%). Even in a deeper region of the cross section (e.g., the region from 800 to 1700 μm) of Fig. 1D, the atomic concentrations of C and N are higher than those of untreated β-TCP, and those of Ca and P are lower, which indicates that plasma-polymerized films were also deposited on the inner pore surfaces of the deep region of the disk. Plasma-treated porous β-TCP disks used for in vivo experiments of this study were treated on both sides (for 30 min each), as discussed before, so we expect the inner pores of those disks are well coated with plasma-polymerized films.
SEM photos of outer surfaces of untreated and plasma-treated porous β-TCP disks are shown in Fig. 2. Plasma polymerization did not cause structural changes in the porous disks. Typical interconnecting channels are shown in photos at 1000× magnification. The deposited polymer is not visible here because its thickness (about 40 nm, as discussed above) is far smaller than the scales of these images.

Effects of plasma treatment on cell behaviors.
First, we confirmed that the plasma treatment enhanced the hydrophilicity of β-TCP, which was originally hydrophobic. As a result, cell suspension dropped on plasma-treated porous disks infiltrated quickly, and the cells therein adhered to the walls of their deep inner pores (Supplementary Movie 1, Supplementary Fig. 1).
Second, we investigated the effects of the plasma treatment on cell adhesion. Green fluorescent protein (GFP)transgenic bone marrow stromal cells (GFP-BMSCs) were harvested from male GFP-transgenic rats. We seeded  www.nature.com/scientificreports/ 5 × 10 3 GFP-BMSCs on the surface of each dense β-TCP disk, incubated them for 30 min to initiate adhesion, and then detached weakly attached cells by centrifugation, as shown in Fig. 3A. Figure 3B shows fluorescence photos of rat BMSCs attached to dense β-TCP disks before and after centrifugation. As shown in Fig. 3C, both cell counts and adhesion rates were significantly higher for the plasma-treated disks than those of the untreated disks. Additionally, we also analyzed morphologies of rat BMSCs attached to dense β-TCP disks. We seeded 5 × 10 3 GFP-BMSCs on the surface of each dense β-TCP disk and incubated them for 3 h for initial adhesion. The cells were then further incubated with additional GM for 24 h. Figure 3D shows fluorescence images of the cells after the 24 h incubation. It is seen there that the morphology of attached cells on the plasma-treated β-TCP disk exhibits a significant increase in the area of cytoplasm (shown in green in the images). These images are used to evaluate the cell areas, cell circularities, defined in Eq. (1), and cell solidities, defined in Eq. (2), for the untreated and plasma-treated disks, which are shown in Fig. 3E. It should be noted that the sample numbers for the untreated and plasma-treated cases are n = 1884 and n = 1440, respectively, for the analysis of Fig. 3E, and the differences in the mean values are confirmed to be statistically significant with unpaired t-test analysis. As we visually observed in Fig. 3C,E shows that the average area of rat BMSCs is larger on the plasma-treated dense β-TCP disk than on the untreated disk (left), suggesting the enhancement of cell spreading on the plasma-treated surfaces. It also shows that the average circularity (center) and solidity (right) are lower on the plasma-treated dense β-TCP disk than on the untreated disk, indicating the presence of membrane protrusions of rat BMSCs on the plasma-treated dense β-TCP disk.
Third, we performed cell proliferation assays. Considering the difference in the initial cell adhesion, we made the initial number of cells the same by seeding different numbers of GFP-BMSCs on plasma-treated and untreated dense β-TCP disks and plotted the cell proliferation curves by serial Cell Counting Kit-8 (CCK-8) assays (Fig. 4A). It was found that the plasma treatment did not influence cell proliferation (Fig. 4B).
Last, to evaluate the overall osteogenesis including cell adhesion, proliferation, and osteogenic differentiation on plasma-treated and untreated dense disks, we seeded 2 × 10 4 GFP-BMSCs on the surface of each dense disk and performed ALP assays after 5 days of osteogenic induction (Fig. 5A). The plasma treatment significantly improved osteogenesis as demonstrated by ALP staining (Fig. 5B) and ALP activity assay (Fig. 5C).

Enhancement of in vivo new bone formation by the plasma treatment. Plasma-treated and
untreated porous β-TCP disks were symmetrically transplanted into circular bone defects of rat calvarial bones. Histological evaluation and micro-CT analysis were performed at 3 and 6 weeks postoperatively (Fig. 6A).
As seen in Fig. 6B, at postoperative 3 weeks, the volume of new bone formed inside the plasma-treated porous β-TCP disk was evaluated and found not to differ essentially from that inside the untreated porous β-TCP disk. However, at postoperative 6 weeks, the volume of new bone formed inside the plasma-treated porous β-TCP disk was significantly higher than that inside the untreated porous β-TCP disk. The 3D-reconstructed image of new bone along with the host calvarial bone revealed abundant new bone formation in and around the plasmatreated porous β-TCP disk (Fig. 6C). In both untreated and plasma-treated groups, nearly one-third of the β-TCP was absorbed for the 3 weeks between the postoperative 3 and 6 weeks (Fig. 6D) with similar rates. Because the initial volumes of the β-TCP disks were essentially the same (about 9.8 mm 3 ), the β-TCP absorption rate was unaffected by the plasma treatment. Figure 7 shows micro-CT slices and the corresponding histological sections of (A) untreated and (B) plasmatreated porous β-TCP disks transplanted into a rat calvarial bone at postoperative 6 weeks. In the micro-CT slices, the white represents β-TCP, the gray represents the rat calvarial bone or newly formed bone, and the black represents soft tissues or the void of space. In the histological sections, the bright pink represents bony tissues, the pale pink represents soft tissues, the white represents the space of decalcified β-TCP or the void of space, and the nuclei of cells are stained in purple. Magnified images near the center and right interface regions of the histological sections are also listed. More bone formation is observed in the plasma-treated porous β-TCP disk than in the untreated disk. The magnified histological images of the interface regions also indicate that the new bone formed in the plasma-treated β-TCP disk has achieved good interface union with the host bone whereas, at the interface between the untreated porous β-TCP disk and the host rat calvarial bone, the host bone is in contact only with soft tissues and has not achieved solid interface union with new bone.

Discussion
In this study, we successfully formed amine-containing carbon polymers on β-TCP artificial bone surfaces by plasma polymerization using a gas mixture of CH 4 , N 2 , and He. This amine modification on β-TCP artificial bone surfaces enhanced in vitro cell adhesion and osteogenic differentiation as well as in vivo bone regeneration. The effects of amine-modified artificial bone surfaces on the tissue ingrowth and enhancement of osteogenic differentiation are considered to be the main mechanisms underlying this high bone regeneration capacity.
In the treatment of large bone defects with artificial bone, the successful introduction of cells and blood vessels at a substantial distance from the host bone remains challenging 26,27 . To treat "critical size" bone defects, pre-loading of bone or vascular-forming cells or vascular transplantation inside artificial bones has been attempted [28][29][30][31] . These methods usually require long and costly pre-treatment. In the present study, we instead chose a "chemical modification" approach and formulated amine-containing plasma polymerization on the outer and inner surfaces of porous artificial bone. The implantation of such plasma-treated artificial bone in a rat calvarial defect model demonstrated early tissue (cells and vessels) ingrowth. The enhanced cell infiltration by plasma treatment is considered to contribute to this early tissue ingrowth.
Amines, as functional groups, are hydrophilic. This is because, in an aqueous medium, amines become protonated and form positively charged functional groups -NH x + (x = 1-3, depending on how many C atoms the center N atom is bonded with), which attract highly polarized water molecules. The present study revealed that  Fig. 1). Notably, the plasma-treated β-TCP absorbed tissue fluid and rapidly became wet, in contrast to non-treated β-TCP, which remained almost completely dry during the implantation (Supplementary Fig. 2).
Although the volumes of new bone formed at postoperative 3 weeks were observed to be similar between the plasma-treated and untreated porous β-TCP disks (Fig. 6B), the histological sections at postoperative 3 weeks revealed abundant infiltrated cells and tissue formation in the plasma-treated disks ( Supplementary Fig. 3). We demonstrated that β-TCP coated with amine-containing plasma-polymerized films enhanced in vitro osteoblastic differentiation and increased the volume of new bone inside the interconnected pores of artificial bones in vivo. Several effects provided by the amine modification must have contributed to this enhanced bone formation.
Amine modification of a surface is known to strengthen cell adhesion by enhancing integrin binding, which is required for osteoblastic differentiation [32][33][34] . In detail, cell adhesion is mainly mediated by the binding of cellular integrins and adhesive proteins such as fibronectin in the extra-cellular matrix. The positive charges of amines can increase the density of fibronectin and change its conformation 35 . These changes in fibronectin strengthen the cell adhesion by increasing the binding to integrins 36,37 and trigger rapid phosphorylation of focal adhesion-associated tyrosine kinase (FAK) 38 , subsequently triggering extracellular signal-regulated kinase (ERK)/ mitogen-activated protein kinase (MAPK) signaling to upregulate Runt-related transcription factor 2 (Runx2), which is a master regulator of osteoblastic differentiation [39][40][41][42][43][44][45] .
The type of change in cell morphology that we observed on the plasma-treated β-TCP, i.e., the increase of cell areas and the decrease of circularity and solidity, is known to facilitate the osteogenic differentiation of rat BMSCs 46 . This is similar to the earlier observation that human mesenchymal stem cells exhibiting a spreading, rather than maintaining round shapes, appear inclined toward an osteogenic lineage 47 . This is considered to be caused by the upregulation of Ras homolog family member A (RHOA), a transcription factor that regulates the actin cytoskeleton and increases osteogenesis [46][47][48] .
The basicity of amines can also improve osteogenesis by increasing the interfacial pH 49 . A high pH environment around implant materials has been reported to enhance osteoblastic differentiation 49,50 .
Our study also showed that the plasma treatment enhanced the osteogenic differentiation without affecting cellular proliferation (Fig. 2B). In general, cellular proliferation and osteogenic differentiation do not necessarily occur simultaneously. Indeed, earlier studies also demonstrated the enhancement of osteogenic differentiation without enhanced cellular proliferation for different types of cells under different conditions 6,51,52 .
The enhanced cell adhesion, change in cell morphology, and possibly the increase of interfacial pH due to the presence of amine groups on β-TCP artificial bone surfaces are thus consistent with, and underlie, the high bone regeneration capacity achieved by the plasma polymerization on the artificial bones.
The major limitation of this study is, however, that we investigated the bone regeneration capacity only with a rat calvarial defect model. The calvaria has a rich blood supply and therefore offers a supportive environment for bone regeneration. A further investigation on bone regeneration under more stringent conditions, e.g., that for malunion of fractures, is desirable. Furthermore, as the size of artificial β-TCP bones designed for the rat calvarial defect model was small, we were only able to evaluate the bone volume with a high-resolution micro-CT, but unable to obtain other important bone parameters such as trabecular numbers and thicknesses or to perform biomechanical tests to evaluate mechanical strengths of the regenerated bone.
Despite such limitations, the findings of this study indicated that the rapid cell infiltration into the interconnected pores of artificial bones and the enhanced osteoblastic differentiation capability due to the presence of plasma-polymerized films on the artificial bone surfaces contributed to the early tissue ingrowth and high bone regeneration inside and around the plasma-treated artificial bones. Considering the fact that no commercial artificial bone is currently available that possesses a satisfactory osteogenic capacity, we expect these characteristics of amine-modified artificial bones to pave the way to the development of a safe and more effective treatment of large bone defects. The average numbers of cells attached to each dense β-TCP disk after initial adhesion but before centrifugation (left), those after centrifugation (center), and the adhesion rates (right) for untreated and plasma-treated dense β-TCP disks. The data for C are expressed as mean ± SD (n = 5). *p < 0.05, ** p < 0.01. Mann-Whitney U test. Cell morphologies of rat BMSCs attached to dense β-TCP disks were also analyzed after 3 h incubation for the initial adhesion and subsequent 24-h incubation with additional GM. (D) Fluorescence photos of the rat BMSCs after the incubation on untreated (left) and plasma-treated (right) dense β-TCP disks. (E) Comparison of cell areas (left), cell circularities, defined by Eq. (1) (center), and cell solidities, defined by Eq. (2) (right), between the untreated and plasma-treated disks. The cell area represents its size and the cell circularity and solidity characterize its shape. The data of E are expressed as mean ± SD with n = 1860 for "untreated" and n = 1440 for "plasma". ****p < 0.0001. T-test.